- Special Issue Article
- Open Access
On the Chemical Origin of the Gap Bowing in (GaAs)_{1−x}Ge_{2x} Alloys: A Combined DFT–QSGW Study
- Giacomo Giorgi^{1}Email author,
- Mark Van Schilfgaarde^{2},
- Anatoli Korkin^{2} and
- Koichi Yamashita^{1}
- Received: 20 November 2009
- Accepted: 17 December 2009
- Published: 7 January 2010
Abstract
Motivated by the research and analysis of new materials for photovoltaics and by the possibility of tailoring their optical properties for improved solar energy conversion, we have focused our attention on the (GaAs)_{1− x}Ge_{2x} series of alloys. We have investigated the structural properties of some (GaAs)_{1− x}Ge_{2x} compounds within the local-density approximation to density-functional theory, and their optical properties within the Quasiparticle Self-consistent GW approximation. The QSGW results confirm the experimental evidence of asymmetric bandgap bowing. It is explained in terms of violations of the octet rule, as well as in terms of the order–disorder phase transition.
Keywords
- Photovoltaics
- III–V IV-doped alloys
- Bandgap bowing
- Order–disorder phase transition
- DFT
- Quasiparticle Self-consistent GW
Introduction
The design of semiconductors with controlled bandgaps E_{G}, unit cell parameters, and low defect concentration is the ultimate aim in several important areas of industrial applications—electronics, photonics, light-emitting devices, and photovoltaics (PV). Efficient collection of solar energy requires materials that absorb light from different portions of the solar spectrum, followed by efficient conversion into electrons and holes at p–n junctions. A natural approach to the design of new semiconductors is to alloy two materials with similar lattice parameters but different bandgaps. For example, Ge (E_{G} = 0.67 eV [1] at 300 K) and GaAs (E_{G} = 1.43 eV [1] at 300 K) have very similar lattice parameters, 5.649 and 5.66 Å, respectively [2, 3]. There is thus the appealing possibility that (GaAs) _{1− x}Ge_{2x} alloys with intermediate bandgaps can be realized, in particular one characterized by a direct gap, 1 <E_{G} < 1.4 eV (i.e., the average between the bandgaps of Ge and GaAs), which corresponds to the maximum efficiency solar cell for a single bandgap material [4]. Indeed, several theoretical [5–12] and experimental [13–18] papers have been published on studies of metastable alloys between III–V and IV group semiconductors, formally (III–V) _{1− x}(IV)_{2x} compounds.
A group of such mixed single crystal metastable semiconductors covering a wide composition range was synthesized by vapor phase deposition techniques. Noreika et al. [17] deposited (GaAs)_{1− x}Si_{ x } on GaAs(111) by the reactive rf sputtering technique, and they reported an optical bandgap at room temperature of about 1.28 eV for (GaAs)_{0.45}Si_{0.55}. Baker et al. [18] measured the Raman spectra of (GaSb)_{1− x}Ge_{ x } alloys, and found both GaSb- and Ge-like optical modes. The Ge-like mode frequency depends on the alloy’s composition within about 40 cm^{−1}, whereas the GaSb-like mode does not.
(III–V)–IV alloys such as (GaAs)_{1− x}Ge_{2x}, characteristically display a large negative, V-shaped bowing of E_{G} as a function of the alloy composition x. A minimum value of ~0.5 eV was detected by Barnett et al. [13] at a Ge concentration of about 35%, corresponding to the critical value (x_{c}) for phase transition between an ordered zincblende (ZB) and a disordered diamond structure. In the ordered GaAs-rich phase, Ga and As preferentially form donor–acceptor pairs, whereas in the Ge-rich phase, they are randomly distributed in the alloy forming a mixture of n- type (As in Ge) and p- type (Ga in Ge) semiconductors. This phase transition has been put forward to explain [19] the large bowing. Several models have been developed for the ZB → diamond phase transition [8, 19–26]. The stochastic model by Kim and Stern [22] well reproduces this phase transition along the <100> direction at x_{c} = 0.3. However, it poorly describes the growth along the <111> direction, with accumulation of Ge on alternate {111} planes. In general, kinetic models seem to be more appropriate descriptors of the ZB—diamond phase transition than thermodynamic ones: the latter do not take into account the nonuniqueness of the critical composition x_{c} as a function of kinetic growth; they require as input the critical concentration at which the transition takes place, but no restrictions on the formation of Ga–Ga and As–As bonds are imposed. Other models based on the percolation method [26] lead to ZB → diamond transition at x_{c} = 0.57; percolation theory also does not account for different growth conditions. Rodriguez et al. [8] reported that the growth direction and avoidance of “bad bond” formation (i.e., Ga–Ga and As–As bonds) (long-range order, LRO) effects are the main factors responsible for atomic ordering in (GaAs)_{1− x}Ge_{2x} alloys. According to the same model, E_{G} is influenced only by nearest neighbor (NN) atomic interactions (short-range order, SRO) effects. In an extension of the stochastic model of growth along the <100> direction, Holloway and Davis [23, 24] formulated a model for alloys grown in the <100> and <111> directions. SRO effects are common for these two directions. In contrast, the impact of LRO is quite different: a tendency to convert to <111> As growth is predicted [24] as a consequence of the instability of the growth in the <111> Ga direction. In a previous paper [25], the same authors note that the transition from ZB to diamond does not affect the energy gap of (GaAs)_{1− x}Ge_{2x}: this model predicts a critical concentration for the order–disorder transition with x_{c} = 0.75, without any dependence on the method of growth. SRO and LRO effects on the electronic properties of many other IV-doped III–V alloys have also been compared by combining the special quasirandom structures (SQS) and the simulated-annealing (SA) methods for cells of various sizes in conjunction with an empirical pseudopotential approach [27]. In particular, the direct bandgaps of ideal random Al_{1− x}Ga_{ x } As, Ga_{1− x} In_{ x }P, and Al_{1− x} In_{ x } As alloys were studied. SRO effects are reported to increase the optical bowing of the direct bandgap.
Surface faceting has also been detected in these systems, reported to take place with a subsequent phase separation between the GaAs-rich ZB and Ge-rich diamond region during the growth on (001)-oriented GaAs substrates [15]. A direct consequence attributable to the faceting is the bandgap narrowing of such (GaAs)_{1− x}Ge_{2x} (0 <x < 0.22) alloy layers grown by low-pressure metal–organic vapor phase epitaxy. A similar phenomenon has been reported only once previously, for InAs_{ y }Sb_{1− y} grown by molecular beam epitaxy grown at low temperature (T_{g}) [28]. It has been also demonstrated that growth temperature [16] strongly affects the nature of the alloy. (GaAs)_{1− x}Ge_{2x} layers have been epitaxially grown on GaAs (100) substrates at different temperatures. Transmission electron microscopy analysis revealed that at T_{g} = 550°C, Ge separated from GaAs into domains of ~100 Å. Single-phase alloys are detected differently at T = 430°C.
In spite of considerable recent research in novel complex materials for photovoltaics, the relationship between chemical and optical properties of III–V–IV alloys and similar materials is still unknown, and is a matter of current debate. In the present paper, we investigate the chemical nature of the bowing in (GaAs)_{1− x}Ge_{2x} alloys. In particular, we theoretically investigated the structural and optical properties of four different intermediate structured compounds that range between “pure” GaAs and “pure” Ge (x_{Ge} = 0.25, 0.50 (two samples), 0.75).
Computational Details
We performed calculations by using density-functional theory (DFT), within both the local-density approximation (LDA) [29, 30] and the generalized gradient approximation (GGA) of Perdew and Wang [31–33]. We used Blöchl’s all-electron projector-augmented wave (PAW) method [34, 35], with PAW potentials with d electrons in the semicore for both Ga and Ge. Cutoff energies of 287 and 581 eV were set as the expansion and augmentation charge of the plane wave basis. The force convergence criterion for these models was 0.01 eV/Å. The initial (GaAs)_{1− x}Ge_{2x} models consisting of eight atoms were optimized with a 10^{3} Γ- centered k-points sampling scheme.
All the total energy calculations were also performed with the generalized full-potential LMTO method of Ref. [36]. Calculated structural properties and heats of reaction predicted by the two methods were almost identical, indicating that the results are well converged.
It is expected that LDA and GGA predict reasonable heats of reaction of the type in Eq. 1, since reactions involve rearrangement of atoms on a fixed (zincblende) lattice, and there is a large cancelation of errors. Optical properties are much less well described. The LDA is well known to underestimate semiconductor bandgaps, and moreover, the dispersion in the conduction band is poor. In Ge, the LDA gap is negative and Γ_{1c} is lower than L_{1c} in contradiction to experiment. Also the Γ-X dispersion is often strongly at variance with experiment: in GaAsX_{1c−}Γ_{1c} is about twice the experimental value of 0.48 eV.
When considering (GaAs)_{1− x}Ge_{2x} alloys, any of the three points (Γ, X, L) may turn out to be minimum-gap points, so all must be accurately described. Thus, the LDA is not a suitable vehicle for predicting optical properties of these structures.
It is widely recognized that the GW approximation of Hedin [37] is a much better predictor of semiconductor optical properties. The GW approximation is a perturbation theory around some noninteracting Hamiltonian H_{0}; thus the quality of the GW result depends on the quality of H_{0}. It is also important to mention that for reliable results, care must be taken to use an all-electron method [38]. We adopt here a particularly reliable all-electron method, where not only the eigenfunctions are expanded in an augmented wave scheme, but the screened coulomb interaction W and the self-energy Σ = iGW are represented in a mixed plane wave and molecular orbital basis [39, 40]. All core states are treated at the Hartree–Fock level.
Left, LDA calculated bandgaps (LMTO [36], Spin–Orbit effects included) for Γ, X L points for GaAs and Ge Right, QSGW bandgaps for the same points in Ge and GaAs (eV, 0 K), compared with measured values at 0 K. The self-energy was scaled by a factor 0.8, as described in the text. Raw (unscaled) QSGW levels are slightly larger than experiment
LDA BANDGAP (eV) | QSGW BANDGAP (eV) | ||||||||
---|---|---|---|---|---|---|---|---|---|
Γ | L | X | Γ | L | X | ||||
QSGW | Exp | QSGW | Exp | QSGW | Exp | ||||
GaAs (dir.) | 0.23 | 0.75 | 1.43 | 1.47 | 1.52^{a} | 1.73 | 1.80^{a} | 1.84 | 1.98^{a} |
Ge (indir) | −0.22 | −0.04 | 0.55 | 0.94 | 0.90^{b} | 0.74 | 0.74^{b} | 1.06 | 1.09^{b} |
Results
The energy difference (ΔE, per unit, eV) between ZB and WZ polymorphs of GaAs, lattice constant, a, and bulk moduli B(GPa) of GaAs (ZB) and Ge (diamond)
GaAs (ZB) 216, F-43 m, Z = 4 | GaAs (WZ) 186, P 63 mc, Z = 2 | Ge (cubic) 227, Fd-3m, Z = 8 | |
---|---|---|---|
This study, PAW/LDA | |||
ΔE | – | +0.06 | – |
B | 66.14 | 71.8 | |
Lattice constant (Å) | a = 5.605 | a = 3.917, b = 3.886c = 6.505 | a = 5.612 |
This study, PAW/GGA | |||
ΔE | – | +0.03 | – |
B | 79.01 | 71.0 | |
Lattice constant (Å) | a = 5.739 | a = 4.040, c = 6.668 | a = 5.747 |
Previous study (LDA) | |||
ΔE | – | +0.0120^{a} | |
B | 75.7^{b}, 77.1^{e} | 73.3^{c}, 79.4^{c} | |
Lattice constant (Å) | a = 5.654^{a}, 5.53^{b}5.508^{e}, 5.644^{k} | a = 3.912, c = 6.441^{a}a = 3.912, c = 6.407^{b} | a = 5.58^{c}, 5.53^{c} |
Previous study (GGA) | |||
B | 59.96^{h} | 55.9^{c} | |
Lattice constant (Å) | a = 5.74^{h}, 5.722^{i} | a = 3.540, c = 6.308^{l} | a = 5.78^{c} |
Experimentally | |||
ΔE | – | +0.0117^{k} | |
B | 77^{f} | 75^{d} | |
Lattice constant (Å) | a = 5.649^{f}, 5.65^{g} | a = 5.678^{j}, 5.66^{d} |
As seen from Table 2, the LDA generates structural properties closer to experiment than GGA in this context. Thus, we use LDA to study structural properties. Both Ga–As and Ge–Ge bond lengths are 2.43 Å in their most stable polymorph.
At first, we performed an analysis of the Ge dimer in bulk GaAs, at site positions (1/4, 1/4,1/2) and (0,1/2,3/4). We denote this as “alloy model I”, the dimer in an 8-atom GaAs cell with lattice vectors (100), (010), and (001) before relaxation. It can be considered a highly concentrated molecular substitutional Ge_{2} defect in GaAs, for which we predict stability owing to the donor–acceptor self-passivation mechanism.^{1} The first layer of I consists only of As; the second and the third layers (along [001]), are Ge–Ga, and Ge–As, respectively. The fourth is pure Ga. Then, the overall sequence is a repeated “sandwich-like” structure, ···/As/Ge–Ga/Ge–As/Ga/···. The bond lengths were calculated to be 2.38 (Ga–Ge), 2.42 (Ge–Ge), 2.44 (Ga–As), and 2.47 Å (Ge–As)—relatively small variations around the calculated values in bulk Ge and GaAs (2.43 Å). This is perhaps not surprising as the electronic structure can roughly be described in terms of nearly covalent two-center bonds [electronegativity χ = 1.81, 2.01, and 2.18, for Ga, Ge, and As, respectively (http://www.webelements.com)]. In the alloy I the number of “bad bonds” [7, 8], i.e., the number of III–IV and IV–V nearest neighbors, is 12, or 37.5% of the total. According to the Bader analysis [57–59], in the pure host, the difference in electronegativity is responsible for charge transfer from cation to anion. In the alloy formation process, the introduction of Ge reduces the ionic character of the GaAs bond, while increasing the ionic character of the Ge–Ge bond. When a Ge dimer is inserted in GaAs, 0.32 electrons are transferred away from Ge_{Ga} site, while Ge_{As} gains 0.21 electrons The charge deficit on Ga, is reduced from 0.6 electrons in bulk GaAs to 0.47e, while the charge excess on As is reduced from 0.6 to 0.5e. ΔE for reaction Eq. (1) was 0.55 eV, and the optimized lattice parameter was a = 5.621 Å. We have also considered Ge donors (Ge_{Ga}) and acceptors (Ge_{As}) in the pure 8-atom GaAs host cell, separately. The formation energy has been computed according to the Zhang–Northrup formalism [60]. In particular, we calculate ΔE to be 1.03 eV for Ge_{Ga} and 0.84 for Ge_{As}. The sum of the single contributions (1.87 eV) is larger than the heat of formation of the dimer, structure I (0.55 eV). Two reasons explain this difference in energy. First, in the I model alloy, at least one correct bond III–V is formed while in the separate Ge_{Ga} (IV–V) and Ge_{As} (IV–III) cases only bad bonds are formed. The isolated Ge_{Ga} is a donor; the isolated Ge_{As} is an acceptor. Neither is stable in their neutral charged state. We have tested it in a previous analysis (see Footnote) where we calculated +1 and −1 as the most stable charged state for Ge_{Ga} and Ge_{As}, for almost the range of the electronic chemical potential, μ_{e}. These two charged states are indeed formally isoelectronic with the host GaAs. That the stabilization energy 1.87–0.55 = 1.33 eV is only slightly smaller than the host GaAs bandgap establishes that the pair is stabilized by a self-passivating donor–acceptor mechanism.
We considered two alternative structures for the x_{Ge} = 0.50 case. In the IIa structure, Ge atoms are substituted for host atoms at (1/2, 0, 1/2), (1/2, 1/2, 0), (3/4, 3/4, 1/4), and (3/4, 1/4, 3/4); then the lattice was relaxed. It results in a stacking ···/Ga–Ge/Ge–As/··· along <001>. The three cubic directions are no longer symmetry-equivalent: the optimized lattice parameters were found to be a = 5.590 Å, b = c = 5.643 Å. The four intralayer bond lengths were calculated to be Ga–Ge (2.39 Å), Ge–As (2.48 Å), Ge–Ge (2.42 Å), and Ga–As (2.44). Because of the increased amount of Ge, structure IIa was less polarized than I, as confirmed by the slightly more uniform bond lengths. In IIa alloy, the number of “bad bonds” is 16 (i.e., 50%) and ΔE rises to 0.72 eV. In the IIb structure, Ge atoms are substituted for host atoms at (1/4, 1/4, 1/4), (1/4, 3/4, 3/4), (3/4, 3/4, 1/4), and (3/4, 1/4, 3/4). This structure consists of a stack of pure atomic layers, ···/Ga/Ge/As/Ge···, and thus it contains only nearest neighbors of the (Ga–Ge) and (Ge–As) type: thus all bonds are “bad bonds” in this IIb compound. Bond lengths were calculated to be 2.40 Å and 2.49 Å, respectively, and optimized lattice parameters were a = c = 5.682, b = 5.560 Å. In this structure, ΔE = 1.40 eV, almost double that of IIa with identical composition. It supports the picture [7, 8] that III–IV and IV–V bonds are less stable than their III–V, IV–IV counterparts.
This result confirmed findings of an analysis of the substitutional defect Ge in GaAs (see Footnote). In that case, we checked the stability of Ge_{2} dimers (donor–acceptor pair formation) versus isolated Ge couples (n- type Ge + p- type Ge) in GaAs matrix in GaAs supercells. We calculate the energy reaction Ge_{2}:GaAs → Ge_{Ga}:GaAs + Ge_{As}:GaAs to be positive, with ΔE = 0.39 eV, and interpret this as the gain of one III–IV (Ga–Ge) and one IV–V (Ge–As) bond and the loss of one IV–IV (Ge–Ge) bond. (Note that the IIb structure corresponds to the high concentration limit of isolated couples.) According to phase transition theory, the symmetry lowering for the two intermediate systems is the fingerprint of an ordered–disordered phase transition [61]. The calculated deviation from the ideal cubic case (c/a = 1) is 0.94 and 2.15% for IIa and IIb models, respectively, confirming energetic instability for the IIb alloy.
The last model, III, [Ge] = 0.75, consists of pure Ge except that Ga is substituted at (0, 0, 0) and As at (1/4,1/4,1/4). The calculated bond lengths were 2.39, 2.43, 2.45, and 2.48 Å for Ga–Ge, Ge–Ge, Ga–As, and Ge–As, respectively. Cubic symmetry is restored: the optimized lattice parameter (a = 5.624 Å) is nearly identical to structure I. Similarly, ΔE is almost the same as I (~0.54 eV). Indeed, I and III are formally the same model with the same concentration (25%) of Ge in GaAs (I) and GaAs in Ge (III) and the same number of bad bonds, 12. By analogy to model I, we have also calculated the formation energy of a single substituted Ge in the cell. We have also made a preliminary calculation of the stability of isolated Ga acceptors (Ga_{Ge}) and As donors (As_{Ge}) versus that of the substitutional molecular GaAs_{Ge2} in Ge pure host (a supercell of 64 atoms see Footnote); for such concentrations (x_{GaAs} = 0.0312 = 1/32 and x_{Ga(As)} = 0.0156 = 1/64), the molecular substitutional GaAs_{Ge2} is only stabilized by 0.057 eV with respect to the separate couple acceptor–donor. This small stabilization for GaAs_{Ge2} compared to isolated Ga_{Ge} and As_{Ge} confirms the expected similar probability of finding a mixture of n- type and p- type semiconductors in the “disordered” Ge-rich phase. For reference states needed to balance a reaction, we used the most stable polymorph, of the elemental compounds i.e., orthorhombic Ga and rhombohedral As [62]. Ga-rich and As-rich conditions have been considered, corresponding to μ_{Ga(As)} = μ_{Ga(As)}^{bulk}, respectively. In the case of the 8-atom cells, the formation energy for Ga_{Ge} and As_{Ge} are 0.26 eV and 0.58 eV, respectively. Thus, the model III alloy stabilizes the isolated III and V substitutionals by 0.30 eV (ΔE(Ga_{Ge}) + ΔE(As_{Ge})−ΔE_{ III }). This energy is 0.4 eV less than the host bandgap, indicating that the stabilization energy is a little more complicated than a simple self-passivating donor–acceptor mechanism, as we found for the Ge molecule in GaAs.
Lattice parameters: a_{exp} obtained by Eq. (2) using experimental lattice parameters; a_{theor} calculated from Eq. (2), but with optimized lattice parameters at the PAW/LDA level for Ge and GaAs; a_{calc} the PAW/LDA optimized lattice parameters for models I, IIa, IIb, and III. (Italic is for values extrapolated as^{3}√V.)
a _{exp} | a _{theor} | a _{calc (PAW/LDA)} | |
---|---|---|---|
GaAs | 5.649^{a} | 5.605 | |
I | 5.651 | 5.607 | 5.621 |
IIa | 5.653 | 5.609 | 5.625 |
IIb | 5.641 | ||
III | 5.655 | 5.610 | 5.624 |
Ge | 5.660^{b} | 5.610 |
QSGW bandgaps for Γ and R in ordered (GaAs)_{1− x}Ge_{2x} alloys
Г | R | |
---|---|---|
GaAs | 1.66 | 1.80 |
I (x = 0.25) | 0.61 | 0.20 |
IIa (x = 0.5) | 0.16 | _{ − }0.41 |
IIb | <0 | <0 |
III (x = 0.75) | 0.23 | _{ − }0.18 |
Ge | 1.04 | 0.74 |
We finally remark on the lack of definitive analysis of the state of the alloy. In particular, the validity of two viewpoints, a probabilistic growth model based on a layer-by-layer deposition that rejects high-energy bond formation (As–As, Ga–Ga) [22] and a thermodynamic equilibrium based on an effective Hamiltonian (but which is able to describe electronic states [63]) needs to be assessed. In thermodynamic models [19], the Boltzmann weight can always be realized regardless of the measurement time; in probabilistic models [21, 22] further equilibration after the atomic deposition is not possible. It is apparent from the results of Figs 4 and 5 that our theoretical alloy models, and optical properties in particular, depend sensitively on the arrangement of atoms in the alloy.
Conclusions
We have focused on the class of (III–V)_{1− x}IV_{2x} alloys, as candidate new materials with applications relevant to photovoltaics. Previous experiments reported an asymmetric (nonparabolic) bowing of the bandgap as a function of the concentration of the III–V and IV constituents in the alloy.
We have built and optimized 8-atom (GaAs)_{1− x}Ge_{2x} ordered compounds, with x ranging from 0 to 1, as elementary models of alloys. For these systems, we have thus employed DFT to determine structural properties and reaction energies, and QSGW to study optical properties. For the more diluted and more concentrated Ge models, I and III, we have predicted stabilizing clustering effects accompanied by a lowering of the products–reactants excess energy. These two systems are symmetric and additionally characterized by an almost identical lattice parameter. In other words, the calculated excess energy of the two intermediate models (IIa and IIb, x_{Ge} = 0.5), clearly showed that the octet rule violation has lead to the final instability of the alloys. In particular, the larger the number of III–IV and IV–V bonds, the larger the instability of the model. We detected a linear relationship between formation energy and number of bad bonds in the alloys. The relevance of this result stems by the fact that for stoichiometric compounds an elementary model Hamiltonian for the energetics of any alloy with equal numbers of Ge cations and anions as function of the number of bad bonds can be developed.
Our QSGW calculations confirm the bowing of the alloy both at the Γ and L points. We also detected direct relationships between optical and mechanical properties: a diminished cohesion for the intermediate alloys (IIb is even almost metallic), with a sensitive reduction in the bandgap was clearly coupled with an increase in lattice parameter and with a reduced symmetry of these two structures. The reduction in symmetry for the intermediate alloys is also considered the fingerprint of an ordered–disordered phase transition for our alloy models.
Footnotes
^{1} We preliminarily performed calculations on the stability of substitutional Ge donor (Ge_{Ga}), acceptor (Ge_{As}), and Ge pairs in GaAs. We have both compared the stability of Ge_{2} molecule and 2Ge isolated in a 64-atom supercell GaAs host. Similarly, we calculated the stability of As_{Ge}, Ga_{Ge}, and GaAs_{Ge2} still in a 64-atom supercell Ge host. For sake of consistency, these calculations were performed at the same level of theory of present calculations (PAW/LDA), with same cutoff, reduced k-point sampling (4^{3}Γ- centered), and force convergence threshold which is reduced up to 0.05 eV/Å.
Declarations
Acknowledgments
This research was supported by a Grant from KAKENHI (#21245004) and the Global COE Program [Chemical Innovation] from the Ministry of Education, Culture, Sports, Science, and Technology of Japan.
Open Access
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.
Authors’ Affiliations
References
- Kittel C: Introduction to Solid State Physics. Wiley, New York; 2005.Google Scholar
- Levinstein M: Handbook Series on Semiconductor Parameters vol 1, 2. World Scientific, London; 1999.Google Scholar
- Wang SQ, Ye HQ: J. Phys.: Condens. Matter. 2002, 14: 9579. COI number [1:CAS:528:DC%2BD38XovVaksrc%3D]; Bibcode number [2002JPCM...14.9579W] COI number [1:CAS:528:DC%2BD38XovVaksrc%3D]; Bibcode number [2002JPCM...14.9579W] 10.1088/0953-8984/14/41/313Google Scholar
- Streetman BG, Banerjee S: Solid State electronic Devices. Prentice Hall, New Jersey; 2000.Google Scholar
- Holloway H: Phys. Rev. B. 2002, 66: 075131. 10.1103/PhysRevB.66.075313View ArticleGoogle Scholar
- Newman KE, Dow JD, Bunker B, Abels LL, Raccah PM, Ugur S, Xue DZ, Kobayashi A: Phys. Rev. B. 1989, 39: 657. COI number [1:CAS:528:DyaL1MXhtVCisr8%3D]; Bibcode number [1989PhRvB..39..657N] COI number [1:CAS:528:DyaL1MXhtVCisr8%3D]; Bibcode number [1989PhRvB..39..657N] 10.1103/PhysRevB.39.657View ArticleGoogle Scholar
- Osorio R, Froyen S: Phys. Rev. B. 1993, 47: 1889. COI number [1:CAS:528:DyaK3sXhtlKltbk%3D]; Bibcode number [1993PhRvB..47.1889O] COI number [1:CAS:528:DyaK3sXhtlKltbk%3D]; Bibcode number [1993PhRvB..47.1889O] 10.1103/PhysRevB.47.1889View ArticleGoogle Scholar
- Rodriguez AG, Navarro-Contreras H, Vidal MA: Phys. Rev. B. 2001, 63: 115328. Bibcode number [2001PhRvB..63k5328R] Bibcode number [2001PhRvB..63k5328R] 10.1103/PhysRevB.63.115328View ArticleGoogle Scholar
- Ito T, Ohno T: Surf. Sci.. 1992, 267: 87. COI number [1:CAS:528:DyaK38XksFKhs78%3D]; Bibcode number [1992SurSc.267...87I] COI number [1:CAS:528:DyaK38XksFKhs78%3D]; Bibcode number [1992SurSc.267...87I] 10.1016/0039-6028(92)91095-SView ArticleGoogle Scholar
- Ito T, Ohno T: Phys. Rev. B. 1993, 47: 16336. Bibcode number [1993PhRvB..4716336O] Bibcode number [1993PhRvB..4716336O] 10.1103/PhysRevB.47.16336View ArticleGoogle Scholar
- Newman KE, Jenkins DW: Superlattices and Microstruct. 1985, 1: 275. COI number [1:CAS:528:DyaL28XkvVGns7g%3D]; Bibcode number [1985SuMi....1..275N] COI number [1:CAS:528:DyaL28XkvVGns7g%3D]; Bibcode number [1985SuMi....1..275N] 10.1016/0749-6036(85)90016-3View ArticleGoogle Scholar
- Bowen MA, Redfield AC, Froelich DV, Newman KE, Allen RE, Dow JD: J. Vac. Sci. Technol. B. 1983, 1(3):747. COI number [1:CAS:528:DyaL3sXkvFChu7c%3D] COI number [1:CAS:528:DyaL3sXkvFChu7c%3D] 10.1116/1.582685View ArticleGoogle Scholar
- Barnett SA, Ray MA, Lastras A, Kramer B, Greene JE, Raccah PM, Abels LL: Electron. Lett.. 1982, 18: 891. COI number [1:CAS:528:DyaL38XmtVGru7w%3D]; Bibcode number [1982ElL....18..891B] COI number [1:CAS:528:DyaL38XmtVGru7w%3D]; Bibcode number [1982ElL....18..891B] 10.1049/el:19820604View ArticleGoogle Scholar
- Alferov ZhI, Zhingarev MZ, Konnikov SG, Mokan II, Ulin VP, Umanskii VE, Yavich BS: Sov. Phys. Semicond.. 1982, 16: 532.Google Scholar
- Norman AG, Olson JM, Geisz JF, Moutinho HR, Mason A, Al-Jassim MM, Vernon M: Appl. Phys. Lett.. 1999, 74: 1382. COI number [1:CAS:528:DyaK1MXhsFWrtbY%3D]; Bibcode number [1999ApPhL..74.1382N] COI number [1:CAS:528:DyaK1MXhsFWrtbY%3D]; Bibcode number [1999ApPhL..74.1382N] 10.1063/1.123557View ArticleGoogle Scholar
- Banerjee I, Chung DW, Kroemer H: Appl. Phys. Lett.. 1985, 46: 494. COI number [1:CAS:528:DyaL2MXhsVWisLc%3D]; Bibcode number [1985ApPhL..46..494B] COI number [1:CAS:528:DyaL2MXhsVWisLc%3D]; Bibcode number [1985ApPhL..46..494B] 10.1063/1.95569View ArticleGoogle Scholar
- Noreika AJ, Francombe MH: J. Appl. Phys.. 1974, 45: 3690. COI number [1:CAS:528:DyaE2cXls1Sgs7k%3D]; Bibcode number [1974JAP....45.3690N] COI number [1:CAS:528:DyaE2cXls1Sgs7k%3D]; Bibcode number [1974JAP....45.3690N] 10.1063/1.1663840View ArticleGoogle Scholar
- Baker SH, Bayliss SC, Gurman SJ, Elgun N, Bates JS, Davis EA: J. Phys.: Condens. Matter. 1993, 5: 519. COI number [1:CAS:528:DyaK3sXhtlaltro%3D]; Bibcode number [1993JPCM....5..519B] COI number [1:CAS:528:DyaK3sXhtlaltro%3D]; Bibcode number [1993JPCM....5..519B] 10.1088/0953-8984/5/5/003Google Scholar
- Newman KE, Dow JD: Phys. Rev. B. 1983, 27: 7495. COI number [1:CAS:528:DyaL3sXktlWjtb8%3D]; Bibcode number [1983PhRvB..27.7495N] COI number [1:CAS:528:DyaL3sXktlWjtb8%3D]; Bibcode number [1983PhRvB..27.7495N] 10.1103/PhysRevB.27.7495View ArticleGoogle Scholar
- Rodriguez AG, Navarro-Contreras H, Vidal MA: Appl. Phys. Lett.. 2000, 77: 2497. COI number [1:CAS:528:DC%2BD3cXntlSqu70%3D]; Bibcode number [2000ApPhL..77.2497R] COI number [1:CAS:528:DC%2BD3cXntlSqu70%3D]; Bibcode number [2000ApPhL..77.2497R] 10.1063/1.1318722View ArticleGoogle Scholar
- Stern EA, Ellis F, Kim K, Romano L, Shah SI, Greene JE: Phys. Rev. Lett.. 1985, 54: 905. COI number [1:CAS:528:DyaL2MXhsFyns74%3D]; Bibcode number [1985PhRvL..54..905S] COI number [1:CAS:528:DyaL2MXhsFyns74%3D]; Bibcode number [1985PhRvL..54..905S] 10.1103/PhysRevLett.54.905View ArticleGoogle Scholar
- Kim K, Stern EA: Phys. Rev. B. 1985, 32: 1019. COI number [1:CAS:528:DyaL2MXkvFKltb0%3D]; Bibcode number [1985PhRvB..32.1019K] COI number [1:CAS:528:DyaL2MXkvFKltb0%3D]; Bibcode number [1985PhRvB..32.1019K] 10.1103/PhysRevB.32.1019View ArticleGoogle Scholar
- Davis LC, Holloway H: Phys. Rev. B. 1987, 35: 2767. COI number [1:CAS:528:DyaL2sXhs1Klsrk%3D]; Bibcode number [1987PhRvB..35.2767D] COI number [1:CAS:528:DyaL2sXhs1Klsrk%3D]; Bibcode number [1987PhRvB..35.2767D] 10.1103/PhysRevB.35.2767View ArticleGoogle Scholar
- Holloway H, Davis LC: Phys. Rev. B. 1987, 35: 3823. COI number [1:CAS:528:DyaL2sXhvVKktLw%3D]; Bibcode number [1987PhRvB..35.3823H] COI number [1:CAS:528:DyaL2sXhvVKktLw%3D]; Bibcode number [1987PhRvB..35.3823H] 10.1103/PhysRevB.35.3823View ArticleGoogle Scholar
- Holloway H, Davis LC: Phys. Rev. Lett.. 1984, 53: 830. COI number [1:CAS:528:DyaL2cXlt1Srsr4%3D]; Bibcode number [1984PhRvL..53..830H] COI number [1:CAS:528:DyaL2cXlt1Srsr4%3D]; Bibcode number [1984PhRvL..53..830H] 10.1103/PhysRevLett.53.830View ArticleGoogle Scholar
- D’yakonov MI, Raikh ME: Fiz. Tekh. Poluprovodn.. 1982, 16: 890. Sov. Phys. Semicond. 16, 570 (1982) Sov. Phys. Semicond. 16, 570 (1982)Google Scholar
- Mader K, Zunger A: Phys. Rev. B. 1995, 51: 10462. COI number [1:CAS:528:DyaK2MXlsVSgtrc%3D]; Bibcode number [1995PhRvB..5110462M] COI number [1:CAS:528:DyaK2MXlsVSgtrc%3D]; Bibcode number [1995PhRvB..5110462M] 10.1103/PhysRevB.51.10462View ArticleGoogle Scholar
- Seong Y, Norman AG, Ferguson IT, Booker GR: J. Appl. Phys.. 1993, 73: 8227. COI number [1:CAS:528:DyaK3sXlt1ymu7w%3D]; Bibcode number [1993JAP....73.8227S] COI number [1:CAS:528:DyaK3sXlt1ymu7w%3D]; Bibcode number [1993JAP....73.8227S] 10.1063/1.353440View ArticleGoogle Scholar
- Perdew JP, Zunger A: Phys. Rev. B. 1981, 23: 5048. COI number [1:CAS:528:DyaL3MXktFejurk%3D]; Bibcode number [1981PhRvB..23.5048P] COI number [1:CAS:528:DyaL3MXktFejurk%3D]; Bibcode number [1981PhRvB..23.5048P] 10.1103/PhysRevB.23.5048View ArticleGoogle Scholar
- Ceperley DM, Alder BI: Phys. Rev. Lett.. 1980, 45: 566. COI number [1:CAS:528:DyaL3cXltlyhtrY%3D]; Bibcode number [1980PhRvL..45..566C] COI number [1:CAS:528:DyaL3cXltlyhtrY%3D]; Bibcode number [1980PhRvL..45..566C] 10.1103/PhysRevLett.45.566View ArticleGoogle Scholar
- Burke K, Perdew JP: Y. Wang. Electronic Density Functional Theory: Recent Progress and New Directions, Plenum Press, New York; 1998.Google Scholar
- Perdew JP: Electronic Structure of Solids 91. Akademie Verlag, Berlin; 1991.Google Scholar
- Perdew JP, Chevary JA, Vosko SH, Jackson KA, Pederson MR, Singh DJ, Fiolhais C: Phys. Rev. B. 1992, 46: 6671. COI number [1:CAS:528:DyaK38XlvFyks7c%3D]; Bibcode number [1992PhRvB..46.6671P] COI number [1:CAS:528:DyaK38XlvFyks7c%3D]; Bibcode number [1992PhRvB..46.6671P] 10.1103/PhysRevB.46.6671View ArticleGoogle Scholar
- Blöchl PE: Phys. Rev. B. 1994, 50: 17953. Bibcode number [1994PhRvB..5017953B] Bibcode number [1994PhRvB..5017953B] 10.1103/PhysRevB.50.17953View ArticleGoogle Scholar
- Kresse G, Joubert D: Phys. Rev. B. 1999, 59: 1758. COI number [1:CAS:528:DyaK1MXkt12nug%3D%3D]; Bibcode number [1999PhRvB..59.1758K] COI number [1:CAS:528:DyaK1MXkt12nug%3D%3D]; Bibcode number [1999PhRvB..59.1758K] 10.1103/PhysRevB.59.1758View ArticleGoogle Scholar
- Methfessel M, van Schilfgaarde M, Casali RA: Electronic Structure and Physical Properties of Solids: The Uses of the LMTO Method, Lecture Notes in Physics 535. Springer-Verlag Berlin; 2000:114.Google Scholar
- Hedin L: Phys. Rev.. 1965, 139: A796. Bibcode number [1965PhRv..139..796H] Bibcode number [1965PhRv..139..796H] 10.1103/PhysRev.139.A796View ArticleGoogle Scholar
- Gomez-Abal R, Li X, Scheffler M, Ambrosch-Draxl C: Phys. Rev. Lett.. 2008, 101: 106404. Bibcode number [2008PhRvL.101j6404G] Bibcode number [2008PhRvL.101j6404G] 10.1103/PhysRevLett.101.106404View ArticleGoogle Scholar
- Kotani T, van Schilfgaarde M: Solid State Commun.. 2002, 121: 461. COI number [1:CAS:528:DC%2BD38XhsFagsbY%3D]; Bibcode number [2002SSCom.121..461K] COI number [1:CAS:528:DC%2BD38XhsFagsbY%3D]; Bibcode number [2002SSCom.121..461K] 10.1016/S0038-1098(02)00028-5View ArticleGoogle Scholar
- Kotani T, van Schilfgaarde M, Faleev SV: Phys. Rev. B. 2007, 76: 165106. Bibcode number [2007PhRvB..76p5106K] Bibcode number [2007PhRvB..76p5106K] 10.1103/PhysRevB.76.165106View ArticleGoogle Scholar
- van Schilfgaarde M, Kotani T, Faleev SV: Phys. Rev. B. 2006, 74: 245125. Bibcode number [2006PhRvB..74x5125V] Bibcode number [2006PhRvB..74x5125V] 10.1103/PhysRevB.74.245125View ArticleGoogle Scholar
- van Schilfgaarde M, Kotani T, Faleev SV: Phys. Rev. Lett.. 2006, 96: 226402. Bibcode number [2006PhRvL..96v6402V] Bibcode number [2006PhRvL..96v6402V] 10.1103/PhysRevLett.96.226402View ArticleGoogle Scholar
- Shishkin M, Marsman M, Kresse G: Phys. Rev. Lett.. 2007, 99: 246403. COI number [1:STN:280:DC%2BD1c%2FnslSqsw%3D%3D]; Bibcode number [2007PhRvL..99x6403S] COI number [1:STN:280:DC%2BD1c%2FnslSqsw%3D%3D]; Bibcode number [2007PhRvL..99x6403S] 10.1103/PhysRevLett.99.246403View ArticleGoogle Scholar
- Chantis AN, van Schilfgaarde M, Kotani T: Phys. Rev. Lett.. 2006, 96: 086405. Bibcode number [2006PhRvL..96h6405C] Bibcode number [2006PhRvL..96h6405C] 10.1103/PhysRevLett.96.086405View ArticleGoogle Scholar
- Viña L, Logothetidis S, Cardona M: Phys. Rev. B. 1984, 30: 1979. Bibcode number [1984PhRvB..30.1979V] Bibcode number [1984PhRvB..30.1979V] 10.1103/PhysRevB.30.1979View ArticleGoogle Scholar
- Lautenschlager P, Garriga M, Logothetidis S, Cardona M: Phys. Rev. B. 1987, 35: 9174. COI number [1:CAS:528:DyaL2sXlt1Wgtbk%3D]; Bibcode number [1987PhRvB..35.9174L] COI number [1:CAS:528:DyaL2sXlt1Wgtbk%3D]; Bibcode number [1987PhRvB..35.9174L] 10.1103/PhysRevB.35.9174View ArticleGoogle Scholar
- Yeh CY, Lu ZW, Froyen S, Zunger A: Phys. Rev. B. 1992, 46: 10086. COI number [1:CAS:528:DyaK38Xms1Wqtrw%3D]; Bibcode number [1992PhRvB..4610086Y] COI number [1:CAS:528:DyaK38Xms1Wqtrw%3D]; Bibcode number [1992PhRvB..4610086Y] 10.1103/PhysRevB.46.10086View ArticleGoogle Scholar
- Wang SQ, Ye HQ: J. Phys.: Condens. Matter. 2003, 15: L197. COI number [1:CAS:528:DC%2BD3sXjsVans7g%3D]; Bibcode number [2003JPCM...15L.197W] COI number [1:CAS:528:DC%2BD3sXjsVans7g%3D]; Bibcode number [2003JPCM...15L.197W] 10.1088/0953-8984/15/12/102Google Scholar
- Kalvoda S, Paulus B, Fulde P: Phys. Rev. B. 1997, 55: 4027. COI number [1:CAS:528:DyaK2sXhtlGhsL4%3D]; Bibcode number [1997PhRvB..55.4027K] COI number [1:CAS:528:DyaK2sXhtlGhsL4%3D]; Bibcode number [1997PhRvB..55.4027K] 10.1103/PhysRevB.55.4027View ArticleGoogle Scholar
- Hellwege KH, Madelung O: Landolt–Börnstein New Series Group III. Springer, Berlin; 1982.Google Scholar
- Singh J: Physics of Semiconductors and their Heterostructures. McGraw & Hill, New York; 1993.Google Scholar
- Arabi H, Pourghazi A, Ahmadian F, Nourbakhsh Z: Phys B: Condens Matter. 2006, 373: 16. COI number [1:CAS:528:DC%2BD28XhtVGitLw%3D]; Bibcode number [2006PhyB..373...16A] COI number [1:CAS:528:DC%2BD28XhtVGitLw%3D]; Bibcode number [2006PhyB..373...16A] 10.1016/j.physb.2005.10.130View ArticleGoogle Scholar
- Wronka A: Mater Sci-Pol. 2006, 24: 726.Google Scholar
- CRC Handbook of Chemistry & Physics. 1997.Google Scholar
- Murayama M, Nakayama T: Phys. Rev. B. 1994, 49: 4710. COI number [1:CAS:528:DyaK2cXit1OnsLc%3D]; Bibcode number [1994PhRvB..49.4710M] COI number [1:CAS:528:DyaK2cXit1OnsLc%3D]; Bibcode number [1994PhRvB..49.4710M] 10.1103/PhysRevB.49.4710View ArticleGoogle Scholar
- Bautista-Hernandez A, Perez-Arrieta L, Pal U: J. F. Rivas Silva, Rev. Mex. Fis.. 2003, 49: 9. COI number [1:CAS:528:DC%2BD3sXhvFWruro%3D] COI number [1:CAS:528:DC%2BD3sXhvFWruro%3D]Google Scholar
- Henkelman G, Arnaldsson A, Jónsson H: Comput. Mater. Sci.. 2006, 36: 354. 10.1016/j.commatsci.2005.04.010View ArticleGoogle Scholar
- Sanville E, Kenny SD, Smith R, Henkelman G: J. Comp. Chem.. 2007, 28: 899. COI number [1:CAS:528:DC%2BD2sXjtFCit78%3D] COI number [1:CAS:528:DC%2BD2sXjtFCit78%3D] 10.1002/jcc.20575View ArticleGoogle Scholar
- Tang W, Sanville E, Henkelman G: J. Phys.: Condens. Matter. 2009, 21: 084204. Bibcode number [2009JPCM...21h4204T] Bibcode number [2009JPCM...21h4204T] 10.1088/0953-8984/21/8/084204Google Scholar
- Zhang S, Northrup J: Phys. Rev. Lett.. 1991, 67: 2339. COI number [1:CAS:528:DyaK3MXms1Ohs7s%3D]; Bibcode number [1991PhRvL..67.2339Z] COI number [1:CAS:528:DyaK3MXms1Ohs7s%3D]; Bibcode number [1991PhRvL..67.2339Z] 10.1103/PhysRevLett.67.2339View ArticleGoogle Scholar
- Landau L: Zh. Eksp. Teor. Fiz.. 1937, 7: 19. COI number [1:CAS:528:DyaA1cXislGk] COI number [1:CAS:528:DyaA1cXislGk]Google Scholar
- Mattila T, Nieminen RM: Phys. Rev. B. 1996, 54: 16676. COI number [1:CAS:528:DyaK2sXnt1Wr]; Bibcode number [1996PhRvB..5416676M] COI number [1:CAS:528:DyaK2sXnt1Wr]; Bibcode number [1996PhRvB..5416676M] 10.1103/PhysRevB.54.16676View ArticleGoogle Scholar
- Bar-Yam Y, Kandel D, Domany E: Phys. Rev. B. 1990, 41: 12869. Bibcode number [1990PhRvB..4112869B] Bibcode number [1990PhRvB..4112869B] 10.1103/PhysRevB.41.12869View ArticleGoogle Scholar